Ó Operative Dentistry, 2011, 36-2, 231-238 Effect of the Curing Method and Composite Volume on Marginal and Internal Adaptation of Composite Restoratives E Souza-Junior M Souza-Regis RC Alonso ´ A Freitas M Sinhoreti L Cunha Clinical Relevance Modulated curing methods were shown to be effective to reduce gap formation in composite restoratives. ´Eduardo Jose Souza-Junior, DDS, MS, Department of Restor- ative Dentistry, Piracicaba Dental School, University of SUMMARY Campinas-UNICAMP, Piracicaba–SP, Brazil The aim of the present study was to evaluate ´Marcos Ribeiro de Souza Regis, DDS, School of Dentistry, the influence of curing methods and composite University of Bahia, Salvador–BA, Brazil volumes on the marginal and internal adapta-Roberta Caroline Bruschi Alonso, DDS, MS, PhD, Department tion of composite restoratives. Two cavities ˜ of Biomaterials, Bandeirante University of Sao Paulo - with different volumes (Lower volume: 12.6 UNIBAN, SP, Brazil mm3; Higher volume: 24.5 mm3) were preparedAnderson Pinheiro de Freitas, DDS, MS, PhD, associate on the buccal surface of 60 bovine teeth and professor, School of Dentistry, University of Bahia, Salva- restored using Filtek Z250 in bulk filling. For dor–BA, Brazil each cavity, specimens were randomly as-Mario Alexandre Coelho Sinhoreti, DDS, MS, PhD, associate signed into three groups according to the professor, Department of Restorative Dentistry-Dental Ma- curing method (n¼10): 1) continuous light (CL: terials Division, Piracicaba Dental School, University of 27 seconds at 600 mW/cm2); 2) soft-start (SS: 10 Campinas-UNICAMP, Piracicaba–SP, Brazil seconds at 150 mW/cm2+24 seconds at 600 mW/*Leonardo Goncalves Cunha, DDS, MS, PhD, associate profes- ¸ cm2); and 3) pulse delay (PD: five seconds at sor, Department of Restorative Dentistry-Dental Materials ´ 150 mW/cm2+three minutes with no light+25 Division, University of Alagoas-FOUFAL, Maceio, AL, Brazil seconds at 600 mW/cm2). The radiant exposure*Corresponding author: BR 101 Norte-Km 97, Tabuleiro for all groups was 16 J/cm2. Marginal adapta- ´ do Martins-Maceio -AL-57072-970, Brazil; e-mail: firstname.lastname@example.org tion was measured with the dye staining gap procedure, using Caries Detector. Outer mar-DOI: 10.2341/10-107-L gins were stained for five seconds and the gap
232 Operative Dentistrypercentage was determined using digital im- niques) are determinant factors with regard toages on a computer measurement program shrinkage stress magnitude.4 Even after light expo-(Image Tool). Then, specimens were sectioned sure, the polymerization reaction continues from fivein slices and stained for five seconds, and the minutes to 24 hours, increasing the degree ofinternal gaps were measured using the same conversion and the volumetric shrinkage and alsomethod. Data were submitted to two-way anal- leading to a significant increase of stress at theysis of variance and Tukey test (p,0.05). Com- tooth/composite interface.5,6posite volume had a significant influence on The cavity configuration (C-factor) was consideredsuperficial and internal gap formation, de- the main determinant of shrinkage stress in com-pending on the curing method. For CL groups, posite restoratives.7 However, Braga and others8restorations with higher volume showed high- showed that the volume of composite is also stronglyer marginal gap incidence than did the lower related to shrinkage stress and microleakage ofvolume restorations. Additionally, the effect of restorations. The higher the composite volume, thethe curing method depended on the volume. greater the amount of monomer to convert and theRegarding marginal adaptation, SS resulted in higher the stress generated on the bonded interface.8a significant reduction of gap formation, when Moreover, previous studies9,10 concluded that, forcompared to CL, for higher volume restora- similar volumes, bulk or incremental filling havetions. For lower volume restorations, there similar results on marginal adaptation.was no difference among the curing methods.For internal adaptation, the modulated curing Shrinkage stress is also regulated by the curingmethods SS and PD promoted a significant protocol. Low light intensity or modulated curingreduction of gap formation, when compared to methods reduce the polymerization rate of compos-CL, only for the lower volume restoration. ites, consequently reducing the stress rate generat-Therefore, in similar conditions of the cavity ed11,12 and improving the marginal adaptation ofconfiguration, the higher the volume of com- composite restoratives.13 In this sense, modulatedposite, the greater the gap formation. In addi- curing methods such as soft-start (SS) and pulsetion, modulated curing methods (SS and PD) delay (PD) have been proposed.7,14-16can improve the interfacial quality of compos- Yoshikawa and others17 reported that the SSite restorations through the reduction of in- curing method promotes better marginal sealing ofternal gaps in lower volume composite cavo-surface margins of composite restoratives. Inrestoratives. addition, this curing method can provide similar properties, such as hardness and residual monomer INTRODUCTION concentration, when compared to the conventionalResin composites have been widely used in direct continuous curing method.18esthetic restorative procedures. However, polymeri- The PD curing method is a variation of the SSzation shrinkage still harms the interfacial quality, protocol. In this method, a lag period ranging fromcreating adaptation problems.1 When this shrinkage 10 seconds to five minutes is utilized between lowtakes place under confinement, as a result of and high light exposure scenarios.19,20 Previousbonding to cavity walls, stresses on the bond studies19,21 have associated this method with re-interface will develop,2 potentially leading to gap duced gap formation through the reduction onformation, marginal pigmentation, and secondary shrinkage stress. Cunha and others11 showed thatcaries. The presence of gaps on the tooth/resin the PD method provided the greatest reduction ininterface is considered the first sign of restoration the stress rate of dental composites, with nofailure.3 significant reduction in the degree of conversion. Although the polymerization shrinkage is the Although several studies1,11,13,17,19,22-24 havecause of adaptation problems of composite restora- pointed out the benefits of the modulated photoacti-tions, it is an inherent characteristic of the composite vation, this issue has not yet been completelyand directly related to the degree of conversion. established as successful. One of the reasons isTherefore, the actual factor to be managed is the because composites behave differently when subject-shrinkage stress generated by the polymerization ed to modulated photoactivation.25 In this sense,shrinkage. some studies showed no positive effect of modulated Composite formulation and volume, curing proto- photoactivation on shrinkage stress26 or gap forma-cols, and restorative procedures (as insertion tech- tion.27-29 In addition, Stansbury and others30 stated
Souza-Junior Others: Curing Methods and Composite Volume on Marginal Adaptation 233that modified photo-curing protocols, including SP, Brazil) mounted in a high-speed hand piecestepped or pulsed irradiation programs, appear to (Kavo, Joinville, SC, Brazil) under constant air-have limited potential to reduce the overall stress water cooling, as follows:developed if comparable levels of conversion areachieved compared to a standard protocol. Also, Lower volume cavity—4 mm diameter31 mm deep,Froes-Salgado and others31 have suggested that ´ volume of 12.6 mm3, prepared using tip #3053.modulated curing methods may also reduce the Higher volume cavity—5 mm diameter31.25 mmoverall degree of conversion, not just the rate, and deep, volume of 24.5 mm3, prepared using tipthis may contribute to the reduced stress. Converse- #4054.ly, several studies5,11,14,24 showed that modulated Diamonds tips were replaced after every fifthcuring methods cause no reduction in the degree of preparation. At the superficial margin, the cavityconversion or in mechanical properties if the energy walls formed a 908 angle with the dentin surfacedose is not reduced. Thus, a definitive answer about plane, while the internal cavity angles were roundedthe effect of modulated curing protocols has not been based on the design of the diamond tip used. If anydetermined; therefore, further evaluation of this sign of pulp exposure was noticed during cavityissue is necessary. preparation, the specimen was discarded. The aim of the present study was to evaluate theinfluence of modulated curing methods and compos- Restorative Procedureite volume on superficial and internal adaptation of Each specimen was restored using an etch-and-rinsecomposite restoratives. The first hypothesis tested adhesive system (Adper Single bond 2, batch #3HR,was that the higher the volume of composite, the 3M/ESPE, St Paul, MN, USA), applied in accordancehigher the gap formation due to shrinkage stress. with the manufacturer’s instructions: the cavity wasThe second tested hypothesis was that modulated etched with 35% phosphoric acid gel (Scotchbondcuring methods can improve the marginal and Etchant, 3M/ESPE) for 15 seconds, rinsed for 10interfacial quality of composite restorations. In seconds, and blot-dried. The adhesive system wasaddition, aiming to compare the studied factors, the applied twice with a five-second interval in between,third hypothesis was that situations related to dried carefully with air for 15 seconds in order tohigher shrinkage stress, such as cavities with higher remove residual solvent (observing a glossy surface),volumes, would experience higher benefits of using and light cured for 20 seconds using a LED curingmodulated curing methods. ˜o unit (Ultrablue IS, DMC, Sa Paulo, SP, Brazil) with a power density of 600 mW/cm2. Both cavities were MATERIALS AND METHODS bulk filled with a hybrid composite (Filtek Z250,Specimen Preparation shade A3, batch #3AM, 3M/ESPE) and teeth were randomly assigned into six groups (n¼10), accordingSixty bovine incisors were selected, cleaned, and to the curing method and composite volume. Curingstored in a 0.5% chloramine T solution at 48C for no methods are described in Table 1, and for this stepmore than a week. Roots were sectioned off 1 mm the same LED curing unit previously described wasunder the cement enamel junction using a double- used, with a radiant exposure of around 16 J/cm2, for ˜oface diamond saw (K. G. Sorensen, Sa Paulo, SP, all curing methods. The power density was frequent-Brazil). The buccal surface was ground on a water-cooled mechanical polisher (Metaserv 2000, Buehler,UK Ltd, Lake Bluff, IL, USA) using 80-, 180-, 320-, Table 1: Curing Methods Used in the Present Studyand 600-grit silicon carbide (SiC) abrasive paper(Carbimet Disc Set, #305178180, Buehler, UK Ltd) Curing Method Power Density and Time Exposurein order to expose a flat dentin area of at least 8 mm.These teeth were observed on a stereomicroscope Continuous Light 600 mW/cm2 during 27 s(Zeiss, Manaus, AM, Brazil), at 253 magnification, toobserve whether the enamel had been completely Soft-Starta 150 mW/cm2 during 10 sþ600 mW/cm2 during 24 sremoved. Two kinds of cylindrical cavities with different Pulse Delaya 150 mW/cm2 during 5 sþ3 min lightvolumes and the same C-factor (2.0) were prepared offþ600 mW/cm2 during 25 son the flattened surface using cylindrical diamond a The reduction of power density was obtained using neutral density filters. ˜tips (#3053 and #4054; K. G. Sorensen, Sao Paulo,
234 Operative Dentistryly checked by a radiometer (Demetron Research Table 2: Means in % of Marginal Gap Length (StandardCorp, Danbury, CT, USA). Deviation) on Superficial Margins of Cavities with After the light curing procedures, specimens were Different Volumes and Curing Methodsstored in distilled water at 378C for 24 hours andwere then finished under water using 600- and 1200- Continuous Light Pulse Delay Soft-Startgrit SiC sandpaper and polished with 1- and 0.5-lmdiamond pastes using a polish cloth under water. Low Volume 8.62 (1.42) Ab 8.13 (2.43) Aa 7.44 (1.88) AaSpecimens were ultrasonically cleaned for fiveminutes between finishing and polishing steps. High Volume 17.76 (2.64) Aa 9.10 (2.42) Ba 4.70 (0.69) Ca Mean values followed by different small letters in the column and capitalEvaluation of Marginal and Internal letters in the row differ statistically among themselves for the Tukey test at the level of 5%. Values in parentheses represent standard deviations.AdaptationMarginal adaptation was measured using a stainingtechnique. A 1.0% acid red propylene glycol solution formation that was statistically greater compared to(Caries Detector, Kuraray Co., Osaka, Japan) was the cavity with lower volume. No difference wasapplied at the restoration margins for five sec- observed when SS and PD were compared in theonds.14,18,32 Specimens were then rinsed in tap water different volumes. Additionally, no difference amongand gently blow-dried. Digital images of the dyed curing methods was observed for the lower volumerestorations with 2400-megapixel resolution were restorations. Concerning internal adaptation (Tableobtained using a scanner (HP ScanJet G4050, 3), the modulated curing methods SS and PD showedHewlett-Packard Company, Palo Alto, CA, USA). a reduction on gap formation, when compared to CL,The length of the dye-stained gaps along the cavity in lower volume cavities. However, in higher volumemargins was measured (mm) from the images using cavities, no significant difference among curingthe UTHSCSA Image tool software, version 2.0 methods was observed. In addition, from the results(alpha 2_ September 1997), developed by the De- of internal adaptation, it was possible to observe thatpartment of Dental Science at The University of the higher volume cavity group presented gapTexas Health Science Center (San Antonio, TX, formation that was statistically greater comparedUSA). The length of the gap formed was calculated to the cavity with lower volume for the SS and PDas a percentage of the entire margin length. curing methods. For CL, no difference between higher and lower restoration volume was detected. After the evaluation of gap formation at superficialmargins, the restorations were cut in the buccal- DISCUSSIONlingual direction in slices (1 mm thick) using acutting machine (ISOMET 1000, Buehler, UK LTD, An important factor to consider in promoting theLake Bluff, IL, USA) in order to obtain two slices of clinical success of resin composite restorations is aeach restoration. On each slice, Caries Detector was satisfactory marginal and internal adaptation. Theapplied to stain the internal gaps, and the same presence of gaps is considered the first sign ofprocedures described previously were accomplished restoration failure, clinically evidenced by marginalfor the evaluation of the internal adaptation of the staining.13 It has been accepted that a detectablecomposite restorations. The obtained data (marginal marginal gap would lead to interfacial leakage.3,13and internal adaptation) were transformed (arcsineroot x/100) in order to obtain normal distribution and Table 3: Means in % of Gap Length (Standard Deviation)were submitted to two-way analysis of variance and on Internal Margins of Cavities with DifferentTukey tests at 5% significance. Volumes and Curing Methods RESULTS Continuous Light Pulse Delay Soft-StartNone of the curing methods was capable of ensuringa perfect marginal seal of restorations. Table 2 shows Low volume 13.53 (3.18) Aa 5.10 (2.26) Ba 3.96 (1.68) Bathat marginal gap formation in restorations curedusing SS and PD was significantly reduced, when High volume 9.60 (1.52) Aa 9.92 (1.54) Ab 7.24 (1.82) Abcompared to restorations cured using continuous Mean values followed by different small letters in the column and capitallight (CL), in the higher volume cavity group. For letters in the row differ statistically among themselves for the Tukey test at the level of 5%. Values in parentheses represent standard deviations.CL, the higher volume cavity group presented gap
Souza-Junior Others: Curing Methods and Composite Volume on Marginal Adaptation 235Clinically, the bacterial leakage along the adhesive stress. In addition, gap formation at the pulpal wallinterface has been related to a severe pulpal and axiopulpal angles may promote fluid flow in theresponse. dentin tubules, resulting in postoperative sensitivi- In addition to the importance of bacterial leakage, ty.39in vitro microleakage tests have not been accepted as The composite used in the present study, Filtekpredictive of restoration failure, because they can Z250, has high inorganic filler volume content (60%)show overestimated results as a result of dentin and monomeric system based on components with apermeability to low-molecular-weight colorants/ high molecular weight (BisGMA, BisEMA, UDMA),dyes.32 In this sense, evaluating the presence of which leads to a low volumetric shrinkage (aboutgaps is considered to be more reliable because it 2.2%), according to manufacturer’s information.should be considered as the first sign of restoration However, Filtek Z250 presents a high concentrationfailure that can be clinically evidenced by marginal of photoinitiators in order to offer a satisfactory curestaining.3 Thus, the identification of early marginal in 20 seconds of light exposure, leading to a fastchanges could facilitate the prognosis of the longev- photo-curing reaction and, consequently, fast devel-ity/stability of a composite restoration, because it has opment of shrinkage stress.5been accepted that a detectable marginal gap will In addition, the use of bovine teeth could belead to interfacial leakage.32-34 considered a limitation of this study. One may argue Composite shrinkage stress can damage the that using this substrate is not as accurate as usinginterfacial quality of composite restorations, com- human teeth when different interactions betweenpromising the durability of the restorative treat- bonding systems and tooth substrate are compared.ment. In the present study, none of the curing However, in the present study, the adhesive bondingtechniques or employed material volumes was able system and substrate were standardized for allto ensure a perfect sealing of the interfacial margin groups, thereby standardizing the interaction be-of composite restorations. Internal gap formation tween them. The major aim of this study was towas particularly located at pulpal wall and axiopul- evaluate composite characteristics under confine-pal angles, which are problematic areas for compos- ment cured with different methods. Therefore, theite insertion.32 At the pulpal floor, gap formation is observed differences were caused by the testedrelated to difficulty with the adhesion due to an variables: volume of composite and curing method.increase in tubular density and diameter and In this sense, bovine teeth were selected becauseproportional reduction in intertubular dentin.35 This they are a suitable substrate for the type of test used,condition allows the shrinkage stress to overcome they are easier to obtain than human teeth, andthe bond strength. Gap formation on the axio-pulpal their use does not result in ethical problems.angle could be attributed to the difficulty of accom- According to Reeves and others,40 bovine dentin ismodating composite in this region. Indeed, previous an adequate substitute for human teeth in adhesionstudies1,36,37 related the axio-pulpal angle to an area tests. However, it has been observed that it is moreof significant difficulty related to the insertion of difficult to ensure good marginal quality usingcomposite, and this difficulty of composite accommo- bovine dentin, and this fact could explain the highdation could promote a gap between the composite marginal gap values. Considering that, a successfuland the bonding agent/cavity wall, increasing the technique with bovine teeth tends to be even moreprobability of gap formation. successful than can be achieved using human teeth. Additionally, gap formation at these sites is also In addition, the use of bovine incisors has beenrelated to shrinkage vectors, as observed by Chiang supported by several authors.36,39,41and others.38 These authors explained that the In this study, we tested the hypothesis that thecomposite shrinks with an upward movement, which higher the volume of composite, the greater the gapis determined by two conditions: 1) debonding at the formation, and this hypothesis was accepted. How-bottom of the cavity and 2) intact adhesion to the ever, it should be noted that the reduced gapenamel margins. As soon as the debonding occurs, formation associated with lower volume cavitiesthe intact adhesion will cause the upward move- occurred differently depending on the curing methodment. This can be explained by the fact that the employed. For CL groups, marginal gap formationbonding agent usually exhibits a higher bond was greater for higher volume cavities. However, forstrength to enamel than to dentin. Therefore, SS and PD groups, a higher percentage of gapadhesion to the enamel remains intact while the formation was observed in higher volume cavities, tobond to dentin is lost as a result of the contraction internal margins. The reduction in gap formation
236 Operative Dentistryassociated with lower volume cavities can be ex- to Lim and others,19 an initial irradiance of 150plained based on the reduction in shrinkage stress in mW/cm2 is too high to significantly reduce thea lower volume of composite.8 magnitude of shrinkage stress. However, in the The effect of modulated curing methods depends present work, even when using an initial irradianceon the volume of the cavity. In higher volume of 150 mW/cm2, gap formation was significantlycavities, modulated curing methods generated re- decreased when compared to use of the CL curingduction of superficial gap formation, and in lower method. And this gap reduction is attributed to avolume cavities, these methods generated reduction reduction in shrinkage stress due to a slower curing rate.5,11 The low modulus phase (pre-gel stage) isof internal gap formation. Therefore, the second extended, allowing stress to be relieved by polymertested hypothesis was accepted, because modulated flow and deformation.curing methods reduced gap formation, but thisreduction occurs in different modes, depending on Despite the advantageous effects of the modulatedthe volume of the cavity. Considering that, the third curing methods, some concerns have to be addressed.hypothesis, related to a superior benefit of modulat- Studies have pointed out that the efficacy of theseed curing methods in situations of higher shrinkage methods varies according to formulation, whichstress, cannot be accepted. The benefits of modulated limits the results of the present study to the specificmethods occur differently in both cavities. In higher material used.19 Another potential problem is reduc-volume cavities, the benefits occur in the external tion of polymer cross-link density related to modu-margins (marginal gap formation is reduced by lated curing methods,14 which can render themodulated curing methods). However, in lower polymer network more susceptible to degradation.volume cavities, the benefits occur in the internal However, it should be considered that the mainmargins (internal gap formation is reduced by cause of adhesive restoration failure is the debond-modulated curing methods). ing of the composite-tooth interface,12 and it is directly related to gap formation. Thus, even if less For CL, the fast polymerization process decreases cross-link density is formed,14 a similar degree ofthe time allowed for viscous flow and leads to a rigid conversion,7 better bond strength values,7,12 andpolymer matrix in a few seconds.40 So, shrinkage improved marginal adaptation1,13,43 are achieved,stress starts almost immediately after polymeriza- and these benefits can be considered superior to thetion, and a significant part of the shrinkage occurs afore-mentioned problems.after the polymer matrix has reached a significantlevel of rigidity, which causes higher shrinkage CONCLUSIONstress and may culminate in greater gap formation,as observed in the present study. Based on the results, it can be concluded that the higher the volume of composite, the greater the gap The benefits of modulated curing methods have formation. In a general way, exposing the compositebeen related to the increased ability of the composite to CL intensity (600 mW/cm2) during the entireto flow, delaying the pre-gel stage,8 and to reduced irradiation period can damage the bonding interface,stress rates associated with these methods.7 Con- thereby increasing marginal gap formation. Howev-versely to CL photoactivation, this scenario pro- er, none of the curing methods tested were able tomotes a slower formation of the polymer network ensure perfect sealing of margins, although modu-and cross-links, favoring better conditions, compared lated curing methods (SS and PD) could reduce gapto molecular adaptation, within the polymeric chain formation, depending on the volume of the cavity.that has been developed under the cavity confine-ment.42 The low initial intensity employed for these (Accepted 21 October 2010)curing methods could reduce the stress rate andconsequently the stress magnitude of composite REFERENCESrestoratives, causing less damage to the restoration 1. Alonso RCB, Cunha LG, Correr GM, Brandt WC, Correr-margins and improving bond strength.1,11,19,22,42 Sobrinho L Sinhoreti MAC (2006) Relationship betweenAfter this initial step, a complement of the polymer- bond strength and marginal and internal adaptation ofization using high intensity ensures satisfactory composite restorations photocured by different methodsenergy dose to guarantee adequate degree of con- Acta Odontologica Scandinavica 64(5) 306-313.version and mechanical properties. 2. Braga RR, Ballester RY Ferracane JK (2005) Factors involved in the development of polymerization contraction Two modulated curing methods were tested in stress in resin composites: A systematic review Dentalthe present study: SS and PD techniques. According Materials 21(10) 962-970.
Souza-Junior Others: Curing Methods and Composite Volume on Marginal Adaptation 237 3. Hilton TJ (2002) Can modern restorative procedures and wall adaptation on resin composite restorations Dental materials reliably seal cavities? Part 2 American Journal Materials 17(4) 359-366. of Dentistry 15(4) 279-289. 18. Yap AUJ, Ng SC Slow KS (2001) Soft-start polymer- 4. Condon JR Ferracane JL (2000) Assessing the effect of ization: Influence on effectiveness of cure and post-gel composite formulation on polymerization stress Journal shrinkage Operative Dentistry 26(3) 260-266. of American Dental Association 131(4) 497-503. 19. Lim BS, Ferracane JL, Sakaguchi RL Concon JR (2002) 5. Halvorson RH, Erickson RL Davidson CL (2002) Reduction of polymerization contraction stress for dental Energy dependent polymerization of resin-based compos- composites by two-step light-activation Dental Materials ite. Dental Materials 18(6) 463-469. 18(6) 436-444. 6. Cunha LG, Alonso RCB, Souza-Junior EJC, Neves ACEC, 20. Asmussen E Peutzfeldt A (2001) Influence of pulse- Correr-Sobrinho L Sinhoreti MAC (2008) Influence of delay curing on softening of polymer structures Journal the curing method on the post-polymerization shrinkage of Dental Research 80(6) 1570-1573. stress of composite resins Journal of Applied Oral Sciences 16(4) 266-270. 21. Luo Y, Lo EC, Wei SH Tay FR (2002) Comparison of pulse activation vs. conventional light-curing on material 7. Cunha LG, Alonso RCB, Neves ACEC, de Goes MF, adaptation of a compomer conditioned using total-etch or Ferracane JL Sinhoreti MAC (2009) Degree of conver- a self etch technique Dental Materials 18(1) 36-48. sion and contraction stress development of a resin composite irradiated using halogen and LED at two C- 22. Cunha LG, Alonso RCB, Pfeifer CSC, Correr-Sobrinho L, factor level Operative Dentistry 34(1) 24-31. Ferracane JL Sinhoreti MAC (2008) Contraction stress and physical properties development of a resin-based 8. Braga RR, Boaro LCC, Kuroe T, Azevedo CLN Singer composite irradiated using modulated curing methods at JM (2006) Influence of cavity dimensions and their two C-factors levels Dental Materials 24(3) 392-398. derivates (volume and ‘C’ factor) on shrinkage stress development and microleakage of composite restorations 23. Alonso RCB, Cunha LG, Pantoja CAS, Puppin Rontani Dental Materials 22(9) 818-823. RM Sinhoreti MAC (2007) Modulated curing methods— Effect on marginal and internal gap formation of 9. Duarte SJR, Dinelli W da Silva MH (2007) Influence of restorations using different restorative composites Jour- resin composite insertion technique in preparations with nal of Biomedical Material Research. Part B. Applied high C-factor Quintessence International 38(10) 829-835. Biomaterials 82(2) 346-351.10. Duarte SJR Saad JR (2008) Marginal adaptation of 24. Ilie N, Jelen E Hickel R (2009) Is the soft-start Class 2 adhesive restorations Quintessence International polymerization concept still relevant for modern curing 39(5) 413-419. units? Clinical Oral Investigations 15(1) 21-29 Epub11. Cunha LG, Alonso RCB, Correr-Sobrinho L, Ferracane JL ahead of print. Sinhoreti MAC (2007) Modulated curing methods: 25. Pfeifer CSC, Braga RR Ferracane JL (2006) Pulse delay Influence of contraction stress, degree of conversion and curing: Influence of initial irradiance and delay time on push-out bond strength of composite restoratives Journal of Dentistry 35(4) 318-324. shrinkage stress and microhardness of restorative com- posites Operative Dentistry 31(5) 610-615.12. Cunha LG, Alonso RCB, Pfeifer CSC, De Goes MF, ´ Ferracane JL Sinhoreti MAC (2009) Effect of irradiance 26. Bouschlicher MR Rueggeberg FA (2000) Effect of and light source on contraction stress, degree of conver- ramped light intensity on polymerization force and sion and push-out bond strength of composite restoratives conversion in a photoactivated composite Journal of American Journal of Dentistry 22(3) 165-170. Esthetic Dentistry 12(6) 328-339.13. Alonso RCB, Cunha LG, Correr GM, de Goes MF, Correr- 27. Sahafi A, Peutzfeldt A Asmussen E (2001) Soft-start Sobrinho L, Puppin Rontani RM Sinhoreti MAC (2004) polymerization and marginal gap formation in vitro Association of curing methods and low modulus liners on American Journal of Dentistry 14(3) 145-149. marginal adaptation of composite restorations Acta 28. Lopes MB, Costa LA, Consani S, Gonini AJ Sinhoreti Odontologica Scandinavica 62(6) 298-304. MAC (2009) SEM evaluation of marginal sealing on14. Brandt WC, Moraes RR, Correr-Sobrinho L, Sinhoreti composite restorations using different photoactivation MAC Consani S (2008) Effect of different photo- and composite insertion methods Indian Journal of activation methods on push out force, hardness and Dental Research 20(4) 394-399. cross-link density of resin composite restorations Dental 29. Amaral CM, Peris AR, Ambrosano GM Pimenta LA Materials 24(6) 846-850. (2004) Microleakage and gap formation of resin composite15. Feilzer AJ, de Gee AJ Davidson CL (1990) Quantitative restorations polymerized with different techniques Amer- determination of stress reduction by flow in composite ican Journal of Dentistry 17(3) 156-160. restorations Dental Materials 6(3) 167-171. 30. Stansbury JW, Trujillo-Lemon M, Lu H, Ding X, Lin Y 16. Lu H, Stanbury JW Bowman CN (2005) Impact of Ge J (2005) Conversion-dependent shrinkage stress and curing protocol on conversion and shrinkage stress strain in dental resins and composites Dental Materials Journal of Dental Research 84(9) 822-826. 21(1) 56-67.17. Yoshikawa T, Burrow MF Tagami J (2001) A light ´ 31. Froes-Salgado NR, Pfeifer CS, Francci CE Kawano Y curing method for improving marginal sealing and cavity (2009) Influence of photoactivation protocol and light
238 Operative Dentistry guide distance on conversion and microleakage of com- shrinkage evaluation with 3D deformation analysis from posite restorations Operative Dentistry 34(4) 408-414. microCT images Dental Materials 26(4) 223-231.32. Alonso RCB, Correr GM, Cunha LG, Borges AFS, Puppin 38. Chiang YC, Hickel R, Lin CP Kunzelmann KH (2010) Rontani RM Sinhoreti MAC (2006) Dye staining gap Shrinkage vector determination of dental composite by test: An alternative method for assessing marginal gap lCT images Composites Science and Technology 70(6) formation in composite restorations Acta Odontologica 989-994. Scandinavica 64(3) 141-145. 39. Peutzfeldt A Asmussen E (2004) Determinants of in33. Dietschi D, Magne P Holz J (1993) An in vitro study of vitro gaps formation of resin composites Journal of parameters related to marginal and internal seal of Dentistry 32(2) 109-115. bonded restorations Quintessence International 24(4) 40. Reeves GW, Fitchie JG, Hembree JH Jr Puckett AD 281-291. (1995) Microleakage of new dentin bonding systems using34. Alani AH Toh CG (1997) Detection of microleakage human and bovine teeth. Operative Dentistry 20(6) around dental restorations: A review Operative Dentistry 230-235. 22(4) 173-185. 41. Nakamichi I, Iwaru M Fusayama T (1983) Bovine teeth35. Garberoglio R Brannstrom M (1976) Scanning electron as possible substitutes in the adhesion test. Journal of microscopic investigation of human dentinal tubules Dental Research 62(10) 1076-1081. Archives of Oral Biology 21(6) 355-362. 42. Braga RR Ferracane JL (2002) Contraction stress36. Correr GM, Alonso RCB, Puppin-Rontani RM, Correr- related to degree of conversion and reaction kinetics Sobrinho L Sinhoreti MAC (2005) Marginal and Journal of Dental Research 81(2) 114-118. internal adaptation of composite restorations using a 43. Schilke R, Lisson JA, Bauss O Geurtsen W (2000) resin liner on deproteinized substrate Acta Odontologica Comparison of the number and diameter of dentinal Scandinavica 63(4) 227-232. tubules in human and bovine dentine by scanning ¨37. Chiang YC, Rosch P, Dabanoglu A, Lin CP, Hickel R electron microscopic investigation Archives of Oral Biol- Kunzelmann KH (2010) Polymerization composite ogy 45(5) 355-361.